Critical Variables of Solder Paste Stencil Printing
for Micro-BGA and Fine Pitch QFP
Jianbiao Pan, Gregory
Sallade*, David J. Leandri"
Manufacturing Systems Engineering
W. Packer Ave, Bethlehem, PA 18015, USA
Tel: (610) 758-6702 Fax: (610) 758-4886
*Visteon Automotive Systems
Moms Road, Lansdale, PA 19446-6060, USA
Jianbiao Pan is currently a W.D. candidate in the Department of Industrial & Manufacturing Systems Engineering at Lehigh University. His research interests are
in the areas of modeling and optimization of electronics manufacturing processes, CAD/CAPP/CAM, and quality control. He is a member of IEEE,
IMAPS,and SME. Dr. Gregory
Tonkayis Associate Professor in the Department of Industrial and Manufacturing Systems Engineering at Lehigh University. He is the Director of the Electronics Manufacturing Laboratory and Associate Director of the George E. Kane Manufacturing Technology Laboratory. He has authored or co-authored over 25 technical papers. His areas of interest are manufacturing, automation, electronics manufacturing, and engineering education.
Dr. Robert H. Storer is Professor of Industrial and Manufacturing Systems Engineering, and Co-Director of the Manufacturing Logistics Institute at Lehigh University. He received his B.S. in Industrial and Operations Engineering from the University of Michigan in 1979, and M.S. and Ph.D. degees in Industrial and Systems Engineering from the Georgia Institute of Technology in
1982 and 1986 respectively. His interests lie in applied statistics and operations research.
Ron Sallade is currently employed at Cygnus, Inc in the development
ofmedical device manufacture for the Biotechnology industry. Mr. Sallade, formerly employed at the Advanced Manufacturing Technology Division of the Visteon enterprise of Ford Motor Company, has made extensive improvements in manufacturing for the electronics industry in the areas of screen printing and machine vision. Developments in the screen printing arena awarded him Ford's President's Award for Customer Driven Quality as a member of the Worldwide Screen Printing Process Improvement Team. MI. Sallade graduated Magna Cum Laude from the University of Pennsylvania with a Bachelor of Science in Mechanical Engineering and Applied Mechanics.
Dave Leandri is a Manufacturing Engineer in the Manufacturing, Design & Development Department for Visteon Automotive Systems. He holds a B.S. in Ceramic
Engineering and a M.S. in Engineering Science from Penn State University. Currently, he is pursuing a M.S. degree in
Technical Management from the University of
PennsylvanialWharton. For 6 years he worked on hybrid material selection and processing, more recently working
onSMT processing. Prior to joining Ford, Dave worked as a Development Engineer at Ferro Corporation.
Stencil printing continues to be the dominant method of solder deposition in high volume surface mount assembly. Control of the amount of solder paste deposited is critical in the case of fine pitch and ultra-fine pitch surface mount assembly. The process is still not well understood as
indicated by the fact that industry reports 52
-71% SMT defects are related to the solder paste stencil printing process.
The purpose of this paper is to identify the critical variables that influence the volume, area, and height of solder paste deposited. An experiment was conducted to investigate the effects of relevant process parameters on the amount of solder paste deposited for Ball Grid Array (BGA) and Quad Flat Package (QFP)of 5 different pitches ranging from 0.76
mm (30 mil) to 0.3
mm(12 mil). The effects of aperture size, aperture shape, board finish, stencil thickness, solder type,and print speed were examined. The deposited solder paste was measured by
anin-line fully automatic laser- based 3-D triangulation solder paste inspection system. Analysis of Variance (ANOVA) shows that aperture size and stencil thickness are the two most critical variables. A linear relationship between transfer ratio (defined as the ratio of the deposited paste volume to the stencil aperture volume) and area ratio (defined as the ratio of the area of the aperture opening to the area of the aperture wall) is proposed. The analysis indicates that the selection of a proper stencil thickness is the key to controlling the amount of solder paste deposited and that the selection of maximum stencil thickness should be based on the area ratio. The experimental results are shown to he consistent with a
model, which will also be described in this paper.
The need for higher pin count, higher performance, smaller size and lighter weight has driven the development of advanced packages such as Quad Flat Package (QFP), Ball Grid Array (BGA), Chip Scale Package (CSP), and Flip Chip. These high-density packages have had a tremendous impact on board-level assembly. One of the main challenges continues to be the solder paste deposition process and, specifically, controlling the amount of solder paste deposited.
Stencil printing is one of the most cost-effective processes for solder paste deposition and it has been widely used in traditional surface mount assembly. If the process can apply solder balls for BGA, CSP and flip chip assembly, it will accelerate the development and utilization of these advanced packages. However, the solder paste stencil printing process is still not completely understood as
indicated by the fact that industry reports 52
-71% of fine pitch SMT defects are related to the solder paste stencil printing process [l].
The stencil printing process is described as follows: When the squeegee is moved along the stencil surface, it forces the solder paste to roll in front of the squeegee and generate a high pressure. The high pressure injects the solder paste into the stencil aperture, which covers the desired areas of
the pad of the PCB. The stencil is lifted off after the print stroke is finished and the solder paste is left on the pad of the PCB [21.
There are many variables that influence the quality of the stencil printing process, which is measured by the amount and position of solder paste deposited. Figure 1 gives a list of important process variables. Pan [I 11 reviewed the work on investigating the effects of the process variables. Since there are more than 4.5 variables, to identify the critical variables is necessary.
An analytical model of the aperture filling process in solder paste stencil printing was developed [ Z ] . In this model, aperture opening size, stencil thickness and squeegee attack angle are concluded to be three critical variables. The deposited solder volume is independent of the stencil thickness. If the squeegee attack angle is fixed and the seal condition between the squeegee and the stencil remains the same, the relationship between transfer ratio and area ratio is:
T R = C * A A R AAR < a critical value
T R = 1 AAR > a critical value
Where TR is the transfer ratio, which is defined as the deposition volume divided by the aperture volume; C is a constant; AAR is the area ratio, which is defined as the ratio of the area of aperture opening to the area of the sidewall of the aperture.
For a circular (BGA) aperture: ARR = W(2H)
For a rectangle (QFP) aperture: ARR = LW/[Z(L+W)Hl Where R is the radius of the circular aperture;
His the stencil thickness; L is the length of the rectangular aperture; and W is the width of the rectangular aperture.
The critical AAR value is where deposited solder paste volume equals the aperture volume and no excess paste is
scooped. The critical value and constant C can be obtained through experimentation. Note that the critical
AARvalue and constant C depend on the squeegee attack angle and the seal condition between the squeegee and the stencil. The model shows that thicker stencils do not necessarily mean higher solder prints and the selection of maximum stencil thickness should be based on the area ratio.
Apenure sizes & tolerance Aperture geomeuy shape Aperture wall roughness Apenure wall angle Stencil thickness Aspect ratio Area ratio Stencil material Flatness
Pattern size vs. time size
Particle size &distribution Slump
Shear strength Homogeneity
Pale composition Adhesion
Stability and consistency Compatibility with substrate
Print speed Separation speed Snapoff distance Printer alignment Squeegee pressure Downstop distance Print direction Stoke length Wiping of stencil P a l e quantity Printer machine Alignment capability Precision Vision system Repeatability
Printing Parameter controls
Cleanliness Squeegee hardness
Board finish (material) Squeegee angle Size and shape of edge Squeegee length Solder mask height relative to pad
squeegeemerial Pad width relative to apemre width
squeegeetip s t r ~ ~
Figure I . Factors that influence the stencil printing process
The Boa1 of this experiment is to determine which are the critical variables that control the amount of solder paste deposited, to validate the model and to determine the critical AAR value. Based on the model, the previous 1999 IEEUCPMT lnrl EIeCtloniCS Manufacturing Tecimotcgy Sympasiurn
0-7803.55024199 $10.09 01999 IEEE
studies [l-111, and discussions with the engineers at Visteon, six variables were selected for this study. They are
stencil thickness, aperture size, aperture shape, board finish, solder paste type, and print speed. The response variable is the volume, area, and height of solder paste deposited, which was measured by an in-line fully automatic laser- based 3-D solder paste inspection system. Table 1 summaries the variables and their levels for the experiment. Table 2 shows the aperture size of the stencils. Table 3 compares the solder paste characteristics of Type 3 and Type 4.
Stencil thickness 0.1
mm(4 mil) 0.15mm (6 mil)
Solder paste type Type 3 Type 4
Board finish Immersion Ag HASL*
Print speed 2 idsec 8 idsec
ADerture size I .
See Table 2
ISee Figure 2 I
Hot Air Solder Leveling.
Table 3 . Solder Paste SDecification
1No-clean LR 735
*F.O.G. (Fineness of Grind) is a simple test to check for the largest particle/agglomerate size in a paste.
The stencil used for the research was laser-cut from stainless steel. Two stencil thicknesses were selected. One is 0.1 mm
(4mil) and the other was 0.15 mm (6 mil). Both
of the stencils had the same pattern, which included three aperture groups:
Group 1: regular rectangular (QFP) apertures with the widths of 0.38 mm (15 mil), 0.32 mm (12 mil), 0.25 mm (10 mil), 0.2 mm (8 mil), and 0.15 mm (6 mil). Each width had 102 pads in the "parallel to squeegee travel" orientation and 102 pads in the "perpendicular to squeegee travel'' orientation. A total of 1020 pads were evaluated.
Group 2: slant rectangular (QFF') apertures with the widths of 0.38 mm (15 mil), 0.32 mm (12 mil), 0.25 mm (10 mil), 0.2 mm (8 mil), and 0.15 mm (6 mil). Each width had 30 pads in the "45 degrees to squeegee travel" orientation and 30 pads in the "135 degrees to squeegee travel" orientation. A total of 300 pads were evaluated. Note that the distance of aperture-to-aperture is designed much larger than the pitch to make measurement feasible.
Group 3: circular (BGA) apertures with the diameters of 0.38 mm (15 mil), 0.32 mm (12 mil), 0.25 mm (10 mil), 0.2
mm (8 mil), and 0.15 mm (6 mil). Each diameter had 216 pads. Atotal of 1080 pads were evaluated.
The test pattern was designed as a 3 x3 Latin Square so the variability due to the pad positions relative to the squeegee and squeegee travel direction were eliminated. The test pattern is shown in Figure 2. It should be noted that the information about aperture size and shape in this design is confounded because they are all in a block. The other 4 factors: stencil thickness, board finish, solder type, and print speed were designed as a factorial design. Due to the time limit of the use of the printing machine in a production line, only one replication was selected. So a total of 16 boards (2-level 4 factors factorial design) were printed.
.t < ', \ . . \ \ \ \ \ \ \
. . .: : : i r , ,, , I,, ,I, I
:.,::, ,, I r I , , r ,, . : 2 < 8 / / ,, , I , . P , , > , / #
Figure 2. Test Pattern of Stencils and FR-4Boards
/In order to generate comparative data on specified process variables, the remaining process variables were determined based on the engineer's knowledge and experience and limited to the values shown in Table 4.
Printer MPM AP HiE
Squeegee 8 inch metal squeegee blade
with 45 degree Squeegee pressure 8 lb
Down-stop distance 0.0835 inch Snap-off distance On-contact
Separation speed Level 6 (about 0.6-0.9 mm/s)
In order to keep solder paste properties the same for each run, the paste was kneaded 3 times before printing. The reason is that the viscosity of solder paste may change after it was kneaded a different number of times. To get the steady state results, each run printed three times and only the third print was measured because the results of the first two may be unstable. The third board of each run was
measured right after it was printed since a long wait time between print and measurement could cause the solvent of paste to evaporate and result in a lower amount when measured.
A fully automatic solder paste inspection system is currently used for inspection of 0.635 mm (25 mil) QFP components of automobile electronics products. An experiment was conducted to investigate whether the system can be used successfully for measuring 0.4 mm and 0.3 mm pitch QFPs and BGAs . The results indicate that the system is capable of measuring down to 0.3 mm (12 mil) pitch QFPs and 0.5 mm (20 mil) pitch BGAs, but fails for 0.4 mm (16 mil) and 0.3 mm (12 mil) pitch BGAs in this project due to too small solder deposits. Therefore, the data of 0.4 mm and 0.3 mm pitch BGAs was removed in the analysis which will be described in the next section.
OF THE DATA
Effects ofAperture Size and Stencil Thickness
The data were analyzed using AnaIysis of Variance (ANOVA). The ANOVA Table for the volume of solder paste deposited for
QFPapertures is shown in Table 5. It shows that aperture size (pitch) and stencil thickness have statistically significant effects on the volume of solder deposited. It is intuitive that a bigger aperture will result in more volume than a smaller one. One may think that a thicker stencil will deposit more volume than a thinner one too. However, this is not always true. The interaction plot of QFP aperture size and 'stencil thickness in Figure 3 shows that the 0.1 mm (4 mil) stencil deposited more volume than the 0.15 mm (6 mil) stencil at the 0.3 mm
pitch level. The interaction plot of BGA aperture size and stencil thickness in Figure 4. shows that the 0.1 mm stencil deposited more volume than the 0.15 mm stencil at the 0.5 mm pitch and 0.635 mm pitch level. Similar experimental results were reported by Fujiuchi and Toriyama .They found that the bump volume with a stencil thickness of 60 pm is larger than that of a stencil thickness of 80 pm. Another analysis was performed using transfer ratio as the response variable. The ANOVA Table for transfer ratio of
QFP apertures is shown in Table 6, and that of BGA apertures in Table 7. The results indicate that pitch (aperture size) and stencil thickness are still the critical variables since they have larger F-ratios. The interaction plot of QFP shown in Figure 5 illustrates that the transfer ratio of the 0.15 mm stencil increases as the pitch increases, while the transfer ratio of the 0.1 mm stencil remains constant as the pitch increases. The interaction of BGA in Figure 6 illustrates that the transfer ratio of the 0.15 mm stencil increases rapidly as the pitch increases, while that of the 0.1 mm stencil increases slowly as the pitch goes up. The relationship between transfer ratio and area ratio is shown in Figure 7. When AAR is larger than 0.6, the transfer ratio is a constant at about 0.9. When AAR is less than 0.6, the transfer ratio is proportional to the area aspect
ratio. The difference between the model and experimental results can be explained by 2 reasons. The first is that part of the paste is deposited outside of the pads of the PCB due to misalignment between the stencil and the PCB (the stencil aperture are designed the same size as the pad sizes of the PCB). The second is that part of the paste sticks to the inside of the stencil apertures. It was found that if the area ratio of BGA apertures equals that of QFP apertures, the two transfer ratios are also equal. That indicates that the relationship between transfer ratio and area ratio is independent of the aperture shape.
Source Sumof Df Mean F-Ratio
Squares Square Main effect A:Pitch 4.77883 4 1.19471 40964.5 B:Stencil 0.542481 1 0.542481 18600.7 Thickness C:Aperture
I199.09 ~~ T B o a r d Finish 0.0057145 1 0.00571457 195.94 E:Solder Type 0.0001592 1 0.000159239 5.46 F:Print Speed 0.0056206 1 0.00562065 192.72
1999IEEWCPMT Infl Electronics Manufacturing TechnologySymposium 0-7803-5502499 $10.00 01999 IEEE
-0.1 Cr) E v
IE 0.08 0)
Source Sumof Df Mean F-Ratio
Squares Square 5 0.04 Main Effects o_ A:Pitch 45.1981 4 11.2995 760.07
*0.02 B:Stencil 8.72832 1 8.72832 587.11 Thickness C:Aperture Shape 3.8069 3 1.26897 85.36 0.2 0.3 0.4 0.5 0.6 0.7 0.8 Pitch (rnrn) D:Board Finish 1.12135 1 1.12135 75.43 ~~~ ~ E:SolderType
F:Print Sueed 14.11505
1276.80 Figure 3. Interaction plot of QFP aperture size and stencil
thickness. 0.016 0.014 I c 0 +0.1 rnrn stencil I E 0.012 E -I+0.15 rnrn stencil
;;;0.01 E 2 0.008
~:0.004 (I) 0.002 0.4 0.5 0.6 0.7 0.8 Pitch (rnrn)
Figure 4. Interaction plot of BGA aperture size and stencil thickness.
Table 7. ANOVA for BGA Solder Transfer Ratio 1 . .. __
0.2 0.3 0.4 0.5 0.6 0.7 0.8
1999 IEEEKPMT Int'l Electronics ManufacturingTechnology Symposium
0-7803-5502-4/99 $10.00 01999 IEEE
____Figure 5 . Transfer ratio vs. Pitch for QFP apertures
I A--c ~- - I
--& 0.5 0.4 I= 0.3 _ _ _ -___ +-0.1 rnm stencil
-.0.2 -1 -m-0.15 mrn stencil -I 0.1 rn I 0 I 0.4 0.5 0.6 0.7 0.8 Pitch (mrn)
Figure 6. Transfer Ratio vs. Pitch for BGA Apertures
Transfer Ratio vs. Area Ratio
I1 0 .-5 0.8
-0.6 0.4 I- 0.2 0 0 0.2 0.4 0.6 0.8 1 1.2 1.4 1.6 1.8 Area Ratio
Fig. 7 Comparison of the model and experimental results (points: experimental data; line: model)
Effects of Aperture Shape
The plot of the mean of deposited solder volume versus aperture direction is shown in Fi,gre 8. It indicates that perpendicular apertures (longer side of the apertures perpendicular to the squeegee travel direction) deposit
8-9% more volume than parallel apertures, while the volume difference between slant apertures and back slant apertures is much smaller. The actual aperture sizes of the two stencils were measured by a microscope since the information of aperture shape was confounded in this experiment. It was found that the perpendicular apertures were slightly (about 3%) wider than the parallel apertures. There is no statistically significant difference between the slant aperture sizes and the back slant aperture sizes. Deducting the aperture size difference, perpendicular apertures print 5 6 % more volume than parallel apertures. Analysis on the height of solder deposits draws the same conclusion. This is a well known experimental phenomena
[5, 61. It can be concluded that arranging the squeegee 45
degrees with respect to the stencil apertures would decrease the variation of the solder deposits height and volume.
___- -~ ___ -__ -_ -_ 0.048
20.046 -0.0455 - -t % 0.045 0.0445 - A 0.044
-Effects of Solder Paste and Print Speed
The effect of print speed has confused many engineers because conflicting experimental results were reported. Mannan, et al.  found a linear rise in paste height with squeegee velocity during stencil printing. Wilson and Bloomfield [7, 81 reported that no noticeable deterioration in print height occurred in print speeds from 25 mm per second to approaching 200 mm per second.
The ANOVA analysis in Tables 5, 6, and 7 shows that strong interaction between solder paste and print speed exists. The interaction plot of solder paste and print speed for QFP apertures and BGA apertures are shown in Figure 9 and Figure 10. It indicates that the transfer ratio of solder type 3 increases rapidly as the print speed increases while that of solder type 4 decreases a little bit as the print speed increases. It can be concluded that the selection of optimal print speed should be based on solder paste type and the print speed could be used to adjust the volume, area, and height of solder deposits.
0.84Q -.-__._ c
1999 IEEUCPMT lnll Electronics Manufacturing Technology Symposium
0-7803-5502-4/99$10.00 01999 IEEE
HASL. The area of solder paste deposited on HASL boards is found always slightly larger than that on silver boards.
- - - .
__This may be due to the dome shape of HASL boards. The
/smooth surface with immersion silver allows the stencil to
0.69 - seal against the pad of the board and to prevent paste from
0.68 - ?.
'..forming solder bridging.
.=m 0 0.67 - \,
E0.66 (I) 0.65 -n s l
j/a--*Type 4 0.62 * N
5p 0.75 0 2 4 6 8 10 2 +-Immersion silver
Print Speed (idsec) 0.7
0.65 Figure 10. Interaction plot of solder type and print speed for
BGA apertures 0.6
This experimental phenomena may be explained as follows: the amount of solder paste deposited is determined by the aperture opening size and paste pressure generated. The paste pressure is proportional to the viscosity of solder paste times the print speed . Since solder paste is a non- Newtonian fluid, its viscosity changes with the change of shear rate. The high print speed results in a high shear rate so that the viscosity of the paste decreases. The result of the solder viscosity times the print speed depends on the solder rheology (the change in viscosity versus the shear rate). Different solder pastes have different rheologies. This is why an interaction exists between solder paste and print speed.
The most common surface finish of PCB is hot-air solder leveling (HASL). However, the dome of the pad (uneven surface) from HASL can affect the fine pitch solder paste printing [121. Therefore, other surface finishes including immersion deposition are receiving attention these days. A comparison of different board finishes was made by Seto, et al.  and Bratin, et al. . No reports on effects of board finish seem to have been published yet.
The relationship between the transfer ratio of deposited solder paste and the board finish for different pitches of QFP and for BGA are shown in Figure 11 and Figure 12. It indicates that more solder paste was deposited on HASL boards when the area of aperture opening is small (all BGA apertures and 0.3 mm pitch QFP apertures) while more solder paste was deposited on silver boards when the area of aperture opening is big (larger than 0.3 mm pitch QFP apertures). In addition, an interaction between solder type and board finish is found.
One of the important considerations of board finish is flatness of board surface. Generally, boards with immersion silver have a better surface in flatness than boards with
0.2 0.3 0.4 0.5 0.6 0.7 0.8
Figure 11. Transfer ratio vs. board finish for QFP apertures.
-0 0.8 Q E 0.7 0.6 ~-0.5 +-Immersion Silver -bHASL -0.4 0.3
!0.4 0.5 0.6 0.7 0.8 Pitch (mm)
Figure 12. Transfer ratio vs. board finish for BGA apertures
The following conclusions are drawn from our analysis:
1) The most critical process variables influencing the amount of solder paste deposited are aperture size and stencil thickness.
2) The transfer ratio is determined by the area ratio. Thicker stencils do not necessarily mean higher solder prints. The area ratio of larger than 0.6 is recommended for the selection of a proper stencil thickness.
3) A strong interaction between print speed and solder paste type indicates that a proper print speed should be selected depending on the solder paste type.
4) A perpendicular aperture prints higher and more volume than a parallel aperture. Aperture orientation of 1999 IEEOCPMTInt'l Electronics Manufacturing Technology Symposium
45 degrees and 135 degrees with respect to the squeegee can decrease the variation of solder deposits. 5) Small apertures print more on HASL boards and big
apertures print more on immersion silver boards. Solder deposits on HASL boards cover more area than that on immersion silver boards.
Richard S . Clouthier, "The Complete Solder Paste Printing Processes", SMT, Vol. 13, No. 1 (special supplement: Guide to Soldering & Printing), pp. 6-8, 1999.
Jianbiao Pan and Gregory L. Tonkay, "A Study of the Aperture Filling Process in Solder Paste Stencil Printing", will appear in the Proceedings of ASME 1999 International Mechanical Engineering Congress and Exposition, Nashville, Tennessee, 1999.
Jianbiao Pan, G. L. Tonkay, R. H. Store, R. M. Sallade, and D. J. Leandri, "Gauge Repeatability &
Reproducibility Study for a 3-D Solder Paste Inspection System", will appear in the Proceedings of International Symposium on Microelectronics, Chicago,
S . H. Mannan, N. Ekere, N.I. Ismail, and E.K. Lo, "Squeegee Deformation Study in the Stencil Printing of Solder Pasts", IEEE Transactions on Components, Hybrids, and Manufacturing Technology, Vol. 17, No.
3, pp. 470475.1994.
H.W. Markstein, "Controlling the Variables in Stencil Printing", Electronic Packaging & Production, Vol. 37, NO. 2, pp. 48-56, 1997.
 S.H. Mannan, N.N. Ekere, I. Ismail, and E.K. Lo, "Squeegee Deformation Study in the Stencil Printing of Solder Pastes," IEEE Transactions on Components,
Hybrids, and Manufacturing Technology, Vol. 17, No.
3, pp. 470-475, 1994.
 T. Wilson and D. Bloomfield, "An Optimistic Outlook for Ultra Fine Pitch (Part I)," Electronic Production, pp. 39-42, February 1995.
 T. Wilson and D. Bloomfield, "An Optimistic Outlook for Ultra Fine Pitch (Part II)," Electronic Production, pp. 83-86, March 1995.
 S. Fujiuchi, and K. Toriyama, "Collective Screen Printing for Carrier Bump and SMT Pads,"
Proceedings of IEEUCPMT International Electronics Manufacturing Technology Symposium, pp. 109- 1 12,
[lo] W. E. Coleman, "Stencil Design for Advanced Packages," SMT, Vol. 10, No. 6, pp. 34-37, 1996.
[11J Jianbiao Pan, "Modeling and Process Optimization of Solder Paste Stencil Printing for Fine Pitch Surface Mount Assembly," Ph.D. Proposal, Lehigh University, Bethlehem, PA, 1998.
[121 George Trinite, "Importance of Board Planarity," SMT, Vol. 13, No. 1 (special supplement: Guide to Soldering &Printing), pp. 12-13, 1999.
[131 P. Seto, J. Evans and S . Bishop, "Analysis of the Palladium Finish," SMT, Vol. 13, No. 6, pp. 60-63, 1999.
[141 Peter Bratin, Michael Pavlov and Gene Chalyt, "Evaluating Finishes Using SERA," PC FAB, Vol. 22,
NO.5, pp. 30-37, 1999.
1999 IEEVCPMT lnrl Electronics Manufacturing Technology Symposium
0-7803-550249 $10.00 01999 IEEE